Basics of Measuring the Dielectric Properties of Materials
date post
16Oct2014Category
Documents
view
51download
10
Embed Size (px)
Transcript of Basics of Measuring the Dielectric Properties of Materials
Agilent Basics of Measuring the Dielectric Properties of MaterialsApplication Note
ContentsIntroduction ..............................................................................................3 Dielectric theory .....................................................................................4Dielectric Constant ............................................................................4 Permeability........................................................................................7
Electromagnetic propagation .................................................................8 Dielectric mechanisms ........................................................................10Orientation (dipolar) polarization ................................................11 Electronic and atomic polarization ..............................................11 Relaxation time ................................................................................12 Debye Relation .................................................................................12 ColeCole diagram............................................................................13 Ionic conductivity ............................................................................13 Interfacial or space charge polarization ..................................... 14
Measurement Systems .........................................................................15Network analyzers ..........................................................................15 Impedance analyzers and LCR meters .........................................16 Fixtures .............................................................................................16 Software ............................................................................................16
Measurement techniques .....................................................................17Coaxial probe ...................................................................................17 Transmission line ............................................................................20 Free space .........................................................................................23 Resonant cavity ...............................................................................25 Parallel plate ...................................................................................27
Comparison of methods ........................................................................28 References ..............................................................................................30 Web Resources ......................................................................................32
2
Introduction
Every material has a unique set of electrical characteristics that are dependent on its dielectric properties. Accurate measurements of these properties can provide scientists and engineers with valuable information to properly incorporate the material into its intended application for more solid designs or to monitor a manufacturing process for improved quality control. A dielectric materials measurement can provide critical design parameter information for many electronics applications. For example, the loss of a cable insulator, the impedance of a substrate, or the frequency of a dielectric resonator can be related to its dielectric properties. The information is also useful for improving ferrite, absorber, and packaging designs. More recent applications in the area of industrial microwave processing of food, rubber, plastic and ceramics have also been found to benefit from knowledge of dielectric properties. Agilent Technologies Inc. offers a variety of instruments, fixtures, and software to measure the dielectric properties of materials. Agilent measurement instruments, such as network analyzers, LCR meters, and impedance analyzers range in frequency up to 325 GHz. Fixtures to hold the material under test (MUT) are available that are based on coaxial probe, coaxial/waveguide transmission line techniques, and parallel plate.
3
Dielectric Theory
The dielectric properties that will be discussed here are permittivity and permeability. Resistivity is another material property which will not be discussed here. Information about resistivity and its measurement can be found in the Agilent Application Note 136911. It is important to note that permittivity and permeability are not constant. They can change with frequency, temperature, orientation, mixture, pressure, and molecular structure of the material.
Dielectric constantA material is classified as dielectric if it has the ability to store energy when an external electric field is applied. If a DC voltage source is placed across a parallel plate capacitor, more charge is stored when a dielectric material is between the plates than if no material (a vacuum) is between the plates. The dielectric material increases the storage capacity of the capacitor by neutralizing charges at the electrodes, which ordinarily would contribute to the external field. The capacitance with the dielectric material is related to dielectric constant. If a DC voltage source V is placed across a parallel plate capacitor (Figure 1), more charge is stored when a dielectric material is between the plates than if no material (a vacuum) is between the plates.
A t C = C 0 k' C0 = C k' = er' = C0
+
A
V
t
+
+
+
+
+
+ +
+
Figure 1. Parallel plate capacitor, DC case
Where C and C0 are capacitance with and without dielectric, k' = e'r is the real dielectric constant or permittivity, and A and t are the area of the capacitor plates and the distance between them (Figure 1). The dielectric material increases the storage capacity of the capacitor by neutralizing charges at the electrodes, which ordinarily would contribute to the external field. The capacitance of the dielectric material is related to the dielectric constant as indicated in the above equations. If an AC sinusoidal voltage source V is placed across the same capacitor (Figure 2), the resulting current will be made up of a charging current Ic and a loss current Il that is related to the dielectric constant. The losses in the material can be represented as a conductance (G) in parallel with a capacitor (C).
4
II = I c + I l = V ( j wC 0 k'+G ) If G = w C 0 k" , then I = V ( j wC 0 )( k'  j k" ) = V ( j wC0 ) k w = 2 f+
AV
t
+
+
+
+
+
+ +
+
C
G

Figure 2. Parallel plate capacitor, AC case
The complex dielectric constant k consists of a real part k' which represents the storage and an imaginary part k'' which represents the loss. The following notations are used for the complex dielectric constant interchangeably k = k* = er = e*r . From the point of view of electromagnetic theory, the definition of electric displacement (electric flux density) Df is: Df = eE where e = e* = e0er is the absolute permittivity (or permittivity), er is the 1 relative permittivity, e0 36 x 109 F/m is the free space permittivity and E is the electric field. Permittivity describes the interaction of a material with an electric field E and is a complex quantity. k = e = er = er jer'' e0 Dielectric constant (k) is equivalent to relative permittivity (er) or the absolute permittivity (e) relative to the permittivity of free space (e0). The real part of permittivity (er') is a measure of how much energy from an external electric field is stored in a material. The imaginary part of permittivity (er'') is called the loss factor and is a measure of how dissipative or lossy a material is to an external electric field. The imaginary part of permittivity (er") is always greater than zero and is usually much smaller than (er'). The loss factor includes the effects of both dielectric loss and conductivity.
5
When complex permittivity is drawn as a simple vector diagram (Figure 3), the real and imaginary components are 90 out of phase. The vector sum forms an angle d with the real axis (er'). The relative lossiness of a material is the ratio of the energy lost to the energy stored.
tan d = e r' = D =
"
er
1 Q
e r''
er e r'
=
Energy Lost per Cycle Energy Stored per Cycle
Figure 3. Loss tangent vector diagram
The loss tangent or tan d is defined as the ratio of the imaginary part of the dielectric constant to the real part. D denotes dissipation factor and Q is quality factor. The loss tangent tan d is called tan delta, tangent loss or dissipation factor. Sometimes the term quality factor or Qfactor is used with respect to an electronic microwave material, which is the reciprocal of the loss tangent. For very low loss materials, since tan d d, the loss tangent can be expressed in angle units, milliradians or microradians.
6
PermeabilityPermeability () describes the interaction of a material with a magnetic field. A similar analysis can be performed for permeability using an inductor with resistance to represent core losses in a magnetic material (Figure 4). If a DC current source is placed across an inductor, the inductance with the core material can be related to permeability.
L = L0 '
R
'=
L L0
L
Figure 4. Inductor
In the equations L is the inductance with the material, L0 is free space inductance of the coil and ' is the real permeability. If an AC sinusoidal current source is placed across the same inductor, the resulting voltage will be made up of an induced voltage and a loss voltage that is related to permeability. The core loss can be represented by a resistance (R) in series with an in